Download presentation

Presentation is loading. Please wait.

1
**Viscoelastic properties**

Polymers have both ideal elastic and viscous behavior depending on time and temperature.

2
**Ideal (elastic) Solid Hooks Law**

response is independent of time and the deformation is dependent on the spring constant.

3
Ideal Solid

4
**Ideal Liquid h= viscosity de/dt = strain rate**

The viscous response is generally time- and rate-dependent.

5
Ideal Liquid

6
**The behaviour of linear elastic were given by Hooke’s law:**

or The behaviour of linear viscous were given by Newton’s Law: E= Elastic modulus s = Stress e= strain de/dt = strain rate ds/dt = stress rate h= viscosity ** This equation only applicable at low strain

7
**Viscoelastic behavior**

Behaviour of most polymer is in between behaviour of elastic and viscous materials. At low temperature & high strain rate, Polymer demonstrate elastic behaviour, At high temperature & low strain rate, Polymer demonstrate viscous behaviour At intermediate temperatures & rate of strain Polymer demonstrate visco-elastic behaviour

8
**Polymer is called visco- elastic because:**

Showing both behaviour elastic & viscous behaviour Instantaneously elastic strain followed by viscous time dependent strain Load released elastic Load added viscous viscous elastic

9
Maxwell Model

10
Kelvin Voigt Model

11
Burger Model

12
**Static Modulus of Amorphous PS**

Glassy Leathery Rubbery Viscous Polystyrene Stress applied at x and removed at y

16
**Dynamic Mechanical Analysis**

17
**Spring Model g = g0⋅sin (ω⋅t) g0 = maximum strain w = angular velocity**

Since stress, t, is t = Gg t = Gg0sin(wt) And t and g are in phase

18
Whenever the strain in a dashpot is at its maximum, the rate of change of the strain is zero ( g = 0). Whenever the strain changes from positive values to negative ones and then passes through zero, the rate of strain change is highest and this leads to the maximum resulting stress. Dashpot Model

19
Kelvin-Voigt Model

20
**Dynamic (Oscillatory) Testing**

In the general case when the sample is deformed sinusoidally, as a response the stress will also oscillate sinusoidally at the same frequency, but in general will be shifted by a phase angle d with respect to the strain wave. The phase angle will depend on the nature of the material (viscous, elastic or viscoelastic) Input Response where 0°<d<90° stress strain viscosity Gmodulus 3.29

21
**Dynamic (Oscillatory) Testing**

By using trigonometry: (3-1) In-phase component of the stress, representing solid-like behavior Out-of-phase component of the stress, representing liquid-like behavior Let’s define: where: 3.30

22
**Physical Meaning of G’, G”**

Equation (3-1) becomes: We can also define the loss tangent: For solid-like response: For liquid-like response: G’storage modulus G’’loss modulus

23
**Real Visco-Elastic Samples**

24
**Typical Oscillatory Data**

G’ G’’ log G log Rubber G’storage modulus G’’loss modulus Rubbers – Viscoelastic solid response: G’ > G” over the whole range of frequencies

25
**Typical Oscillatory Data**

G’ G’’ log G log Melt or solution G0 Less liquid like G’storage modulus G’’loss modulus More liquid like Polymeric liquids (solutions or melts) Viscoelastic liquid response: G” > G’ at low frequencies Response becomes solid-like at high frequencies G’ shows a plateau modulus and decreases with w-2 in the limit of low frequency (terminal region) G” decreases with w-1 in the limit of low frequency

27
Blend

28
Epoxy

29
**Nylon-6 as a function of humidity**

30
E’storage modulus Polylactic acid E’’loss modulus

31
Tg 87 °C

32
Tg -123 °C (-190 F) Tm 135 °C (275 F)

33
**Polyurethane foam (Tg 160 C)**

G’storage modulus Polyurethane foam (Tg 160 C) G’’loss modulus

35
G’storage modulus G’’loss modulus These data show the difference between the behaviour of un-aged and aged samples of rubber, and were collected in shear mode on the DMTA at 1 Hz. The aged sample has a lower modulus than the un-aged, and is weaker. The loss peak is also much smaller for the aged sample.

36
**Tan d of paint as it dries**

37
**Epoxy and epoxy with clay filler**

39
**Dynamic test of a Voigt solid**

40
**Benefits of Dynamic Testing**

Similar presentations

Presentation is loading. Please wait....

OK

EBB 220/3 PRINCIPLE OF VISCO-ELASTICITY

EBB 220/3 PRINCIPLE OF VISCO-ELASTICITY

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on total parenteral nutrition side Ppt on duty roster software Ppt on information security system Ppt on distributed file system Ppt on web search engines Ppt on central limit theorem formula Convert pdf to ppt online nitro Ppt on historical places in india free download Ppt on circuit breaker testing Free ppt on living and nonliving things